Stainless steel Outokumpu's alloy 254 SMO, possess even greater resistance to chloride pitting and crevice corrosion because of their high molybdenum content (>6%) and nitrogen additions. They possess useful service to seawater applications. Ferritic stainless steels possess a ferrite microstructure like carbon steel, which is a body-centered cubic crystal structure and contain between 10.5% and 27% chromium with very little or no nickel. This microstructure is present at all temperatures, due to the chromium addition, and like austenitic stainless steels are not hardenable by heat treatment. They cannot be strengthened by cold work to the same degree as austenitic stainless steels. They
Martensitic stainless steel and internal clamps). Untempered martensite is low in toughness and therefore brittle. The characteristic body-centered tetragonal martensite microstructure was first observed by German microscopist Adolf Martens around 1890. In 1912, Elwood Haynes applied for a U.S. patent on a martensitic stainless steel alloy. This patent was not granted until 1919. Martensitic stainless steel can be nondestructively tested using the magnetic particle inspection method, unlike austenitic stainless steel. Also in 1912, Harry Brearley of the Brown-Firth research laboratory in Sheffield, England, while seeking a corrosion-resistant alloy for gun barrels, discovered and subsequently industrialized a martensitic stainless steel alloy. The discovery was